Document Detail

 Robust penetrating microelectrodes for neural interfaces realized by titanium micromachining. Jump to Full Text MedLine Citation: PMID:  21360044     Owner:  NLM     Status:  Publisher Abstract/OtherAbstract: Neural prosthetic interfaces based upon penetrating microelectrode devices have broadened our understanding of the brain and have shown promise for restoring neurological functions lost to disease, stroke, or injury. However, the eventual viability of such devices for use in the treatment of neurological dysfunction may be ultimately constrained by the intrinsic brittleness of silicon, the material most commonly used for manufacture of penetrating microelectrodes. This brittleness creates predisposition for catastrophic fracture, which may adversely affect the reliability and safety of such devices, due to potential for fragmentation within the brain. Herein, we report the development of titanium-based penetrating microelectrodes that seek to address this potential future limitation. Titanium provides advantage relative to silicon due to its superior fracture toughness, which affords potential for creation of robust devices that are resistant to catastrophic failure. Realization of these devices is enabled by recently developed techniques which provide opportunity for fabrication of high-aspect-ratio micromechanical structures in bulk titanium substrates. Details are presented regarding the design, fabrication, mechanical testing, in vitro functional characterization, and preliminary in vivo testing of devices intended for acute recording in rat auditory cortex and thalamus, both independently and simultaneously. Authors: Patrick T McCarthy; Kevin J Otto; Masaru P Rao Related Documents : 7270114 - Volumetric and dimensional measurements of vestibular structures in the squirrel monkey.17928854 - Association of the jets of enceladus with the warmest regions on its south-polar fractu...3541644 - Taurine protects hamster bronchioles from acute no2-induced alterations. a histologic, ...20206724 - On the effect of x-ray irradiation on the deformation and fracture behavior of human co...23205174 - The use of a kirschner wire in the treatment of a comminuted le fort i fracture: a case...20809744 - Knee flexion influences periprosthetic bmd measurement in the tibia. suggestions for a ... Publication Detail: Type:  JOURNAL ARTICLE     Date:  2011-3-1 Journal Detail: Title:  Biomedical microdevices     Volume:  -     ISSN:  1572-8781     ISO Abbreviation:  -     Publication Date:  2011 Mar Date Detail: Created Date:  2011-3-1     Completed Date:  -     Revised Date:  - Medline Journal Info: Nlm Unique ID:  100887374     Medline TA:  Biomed Microdevices     Country:  - Other Details: Languages:  ENG     Pagination:  -     Citation Subset:  - Affiliation: School of Mechanical Engineering, Birck Nanotechnology Center, Purdue University, West Lafayette, IN, 47907, USA. Export Citation: APA/MLA Format     Download EndNote     Download BibTex MeSH Terms Descriptor/Qualifier:

From MEDLINE®/PubMed®, a database of the U.S. National Library of Medicine

 Full Text Journal Information Journal ID (nlm-ta): Biomed Microdevices ISSN: 1387-2176 ISSN: 1572-8781 Publisher: Springer US, Boston Article Information Download PDF © The Author(s) 2011 Electronic publication date: Day: 1 Month: 3 Year: 2011 pmc-release publication date: Day: 1 Month: 3 Year: 2011 Print publication date: Month: 6 Year: 2011 Volume: 13 Issue: 3 First Page: 503 Last Page: 515 ID: 3085117 PubMed Id: 21360044 Publisher Id: 9519 DOI: 10.1007/s10544-011-9519-5
 Robust penetrating microelectrodes for neural interfaces realized by titanium micromachining Patrick T. McCarthy1 Kevin J. Otto2 Masaru P. Rao34 Address: +1-951-8275870 mprao@engr.ucr.edu 1School of Mechanical Engineering, Birck Nanotechnology Center, Purdue University, West Lafayette, IN 47907 USA 2School of Biological Sciences and the Weldon School of Biomedical Engineering, Purdue University, West Lafayette, IN 47907 USA 3School of Mechanical Engineering, Birck Nanotechnology Center, Purdue University, West Lafayette, IN 47907 USA 4Department of Mechanical Engineering, University of California-Riverside, A313 Bourns Hall, Riverside, CA 92521 USA

Introduction

Penetrating microelectrode devices, which allow direct and selective recording and stimulation of neural tissues, have provided unprecedented opportunity for enhancing understanding of neurophysiological processes underlying many aspects of human function and behavior (Bak et al. 1990, Gelbard-Sagiv et al. 2008). They have also shown immense promise for restoring neurological functions lost to disease, stroke, or injury (Normann 2007), as exemplified by neural prostheses that have enabled restoration of rudimentary auditory perception (Otto et al. 2008, Otto, Rousche and Kipke 2005a, Otto, Rousche and Kipke 2005b) and control of assistive instrumentation for those with motor dysfunction (Hochberg et al. 2006). However, this technology is still in its formative stages and many challenges remain.

While the improvement of chronic recording reliability remains a key near-term challenge for this emerging technology (Vetter et al. 2004), its eventual maturation into a clinically viable technique for restoring lost neurological function will also require development of devices that are capable of withstanding surgical manipulation by neurosurgeons (Kipke et al. 2008), and are immune to safety hazards associated with fracture-based fragmentation. The intrinsic brittleness of silicon, the material most commonly used for the manufacture of such devices, may ultimately prove limiting in this regard. This brittleness, which arises from the low fracture toughness of silicon, creates non-negligible probability for catastrophic failure by fracture. This has not been a significant concern in the evolution of this technology thus far. However, the potential for device fragmentation within the brain, no matter how small, coupled with the potentially severe consequences associated with such fragmentation in future clinical settings, suggests need for consideration of means for addressing this potential concern.

In addition to potential safety concerns, propensity for fracture of silicon-based microelectrodes may also adversely affect reliability, since fracture often results in complete loss of device functionality. It also places practical constraint on many current silicon devices with regard to the device length that can be reliably inserted, since risk of buckling-related fracture increases with device length, while opportunity for increasing buckling resistance through increased shank cross section area is constrained by potential adverse affects associated with increased insertion damage (Szarowski et al. 2003, Seymour and Kipke 2007). In many animal models, this practical length limitation hampers access to sub-cortical structures and largely precludes extension towards simultaneous recording within precisely-defined cortical and sub-cortical regions. This latter capability is of particular interest, since it may serve as a critical enabler for enhancing understanding of important neural processing networks, such as the corticothalamic loops that underlie auditory, visual, and somatosensory processing (Nicolelis et al. 1995, Fanselow and Nicolelis 1999, Sherman and Guillery 2002, Winer and Larue 1987, Hubel and N. 1972, Nicolelis and Shuler 2001). This, therefore, provides additional impetus to develop penetrating microelectrode devices with greater robustness.

Alternative microelectrode materials systems that have been explored include those based on ceramics (Moxon et al. 2004b), polymers (Lee et al. 2004a, Schuettler et al. 2005, Stieglitz et al. 2000, Rousche et al. 2001), and metals (Motta and Judy 2005, Fofonoff et al. 2004). Ceramics offer only limited benefit relative to silicon, with regard to reliability and safety, since they suffer from similar or greater propensity for fracture (Ward et al. 2009). Recently reported microelectrodes based on polycrystalline diamond show potential for realization of highly flexible, thin cross section devices with sufficient stiffness for cortical penetration (Chan et al. 2009). However, low signal to noise ratio observed during neural recording indicates need for further device refinement. Polymers used thus far possess sufficient toughness to mitigate fracture. However, their low elastic moduli typically require trade-off between device stiffness and functional reliability, since relatively large cross section areas are required to ensure insertion reliability and recording site placement accuracy (Lee et al. 2004b, Suzuki, Mabuchi and Takeuchi 2003, Takeuchi et al. 2004), which increases insertion damage. A number of strategies have been proposed to circumvent this trade-off, including those based on stiffening through incorporation of dissolvable rigid polymer coatings (Suzuki et al. 2003) or internal reinforcements (Lee et al. 2004b, Takeuchi et al. 2005, Takeuchi et al. 2004).

Metals show particular promise for use in microelectrode applications due to their high fracture toughness, which ensures graceful failure via plastic deformation, rather than catastrophic fracture (i.e. devices will bend before they break). This increases safety by minimizing potential for fragmentation, and may also enhance reliability, since potential exists for maintaining device functionality despite overloading. Moreover, when coupled with the moderate to high moduli of metals, this enables realization of robust microelectrodes with small cross section areas, thus facilitating insertion and reducing injury. However, despite these advantageous characteristics, metallic microelectrodes reported to-date suffer from limitations that may constrain their ultimate safety or utility. For example, in the devices demonstrated by Motta and Judy (Motta and Judy 2005), gold coatings were implemented to prevent exposure of the underlying nickel structural backbone to the physiological environment. This may adversely affect safety, due to potential for cytotoxic Ni ion release in the event of coating failure. In the devices demonstrated by Fofonoff et al. (Fofonoff et al. 2004), toxicity concerns were largely alleviated through the use of titanium as a structural backbone. However, opportunity for probing sequentially interconnected neural processing networks with such devices is constrained by reliance upon the Utah Electrode Array geometry, which consists of arrayed electrodes with only single, tip-located recording sites.

We have recently reported preliminary results from the development of titanium-based penetrating microelectrodes that seek to address the above-mentioned limitations (McCarthy et al. 2009). Realization of these devices was fundamentally enabled by recently developed techniques that allow, for the first time, fabrication of high-aspect-ratio micromechanical devices within bulk titanium substrates (Aimi et al. 2004, Parker et al. 2005). Herein, we expand upon this report to detail the design, fabrication, mechanical testing, and in vitro functional characterization of titanium-based microelectrode devices intended for use in acute rat auditory cortex and thalamus recording, both independently and simultaneously. Results from acute in vivo characterization of these devices are also briefly touched upon, but are more fully elaborated elsewhere (McCarthy, Rao and Otto 2011).

Design and fabrication
Design

The microelectrodes produced in this effort were designed to study auditory cortex and thalamus responses within a rat model, both individually and simultaneously. As such, short devices (2 mm shank length) were designed for acute cortical recording, and longer devices (4.9 & 5.4 mm shank lengths) were designed for acute thalamic recording, independently of, or in conjunction with cortex. Both device types were modeled after commercially-available “Michigan” type electrode arrays (A1 × 16–5 mm 100–413, NeuroNexus Technologies, Ann Arbor, MI; Shank length = 5 mm, shank thickness ~ 15 μm, shank width = 33–200 μm (distal & proximal ends of shank, respectively), recording site diameter = 23 μm, & recording site pitch = 100 μm). Each titanium device contained 16 independently addressable circular recording sites, and 18 distinct design variants were developed with differing shank length (2, 4.9, & 5.4 mm), recording site diameter (23 & 40 μm), and pitch (50, 75, 100, & 150 μm). Since optimal designs for the intended applications have yet to be defined, the given variation of these parameters was reflective of the desire to eventually determine the most favorable combination that ensures consistent sampling of discrete neurons within the targeted neural regions with high signal to noise ratio.

Figures 1 and 2 show schematic representations of device design variants for acute auditory cortical and corticothalamic recording, respectively. In all devices, recording sites were connected by 5 μm wide traces (with 9 μm pitch) to remote 100 μm × 100 μm contact pads (with 150 μm pitch) arrayed at the proximal end of the device. In devices with 23 μm diameter recording sites, this resulted in shanks with width that tapered from 48 μm at the recording site closest to the distal end of the shank (i.e. near the sharp tip) to 192 μm at the base. In the 40 μm diameter recording site devices, shank width ranged from 65 to 209 μm. Devices intended for cortical recording were designed with 16 recording sites arrayed from the distal end of the shank. Devices intended for corticothalamic recording were designed with one set of 8 recording sites arrayed within the vicinity of 2 mm from the proximal end of the shank, and an additional set of 8 recording sites arrayed from the distal end of the shank.

Fabrication

The titanium-based microelectrode devices were fabricated from 25.4 ± 7.62 μm thick Ti foil substrates (Gr 1 Ti, 99.7% Ti, Fine Metals Corp, Ashland, VA). The as-received foils were first solvent cleaned by ultrasonic agitation in acetone and isopropanol, respectively, followed by DI rinsing and N2 drying. Next, as shown in Fig. 3, the first 0.6 μm SiO2 dielectric layer was deposited by plasma-enhanced chemical vapor deposition (PECVD) to insulate the subsequent electrical structures from the substrate (Benchmark 800 CVD, Axic Inc, Santa Clara, CA; Process conditions SiO2: 230 mT chamber pressure, 26 W RF power, 200 sccm N2O, 35 sccm 5% SiH4, and 300°C lower electrode temperature). The substrates were then subjected to solvent cleaning, and mounted to 100 mm Si carrier wafers with thermally conductive adhesive tape (9882, 3M Electronics, St. Paul, MN). Recording sites, traces, and contact pads were then patterned via standard photolithographic liftoff techniques with electron beam depositions of 20 nm Ti/500 nm Au (CHA SE-600, CHA Industries, Fremont, CA; Process conditions: 1.0 × 10−6 T base pressure and 1 Å/s deposition rate).

Following metal deposition, the samples were soaked in acetone to release the Ti foils from the carrier wafer and then solvent cleaned. The second dielectric layer, composed of 0.2 μm Si3N4 followed by 0.8 μm of SiO2, was then deposited by PECVD to provide insulation from the surrounding environment (Benchmark 800 CVD, Process conditions Si3N4: 400 mT chamber pressure, 100 W RF power, 100 sccm NH3, 120 sccm 5% SiH4, and 300°C lower electrode temperature). This dual layer stack was chosen to promote adhesion to the underlying Au patterns and minimize stress-induced curvature of the devices arising from intrinsic stresses and thermal expansion mismatch between the deposited film and the underlying Ti substrate.

After completion of the second dielectric layer deposition, the Ti foils were again mounted to 100 mm carrier wafers with thermally conductive tape. The contact and recording site windows were then opened via photolithographic patterning and dry etching of the second dielectric layer (E620 R&D, Panasonic Factory Solutions, Japan; Process conditions: 7.5 mT chamber pressure, 500 W ICP source power, 400 W substrate RF power, and 40.0 sccm CHF3). The photoresist was then stripped and the samples were soaked in acetone to release the Ti foils from the carriers.

The third dielectric layer, composed of 0.2 μm Si3N4 and 3.00 μm SiO2, was then deposited by PECVD to serve as an etch mask for the subsequent deep etch of the underlying Ti substrate. The samples were re-mounted to carrier wafers, and the shank profiles were patterned and transferred into the dielectric layers via dry etching (E620 R&D, Process conditions: 1.9 mT chamber pressure, 900 W ICP source power, 200 W substrate RF power, and 40.0 sccm CHF3). The photoresist was then stripped and the shank profiles were transferred through the underlying Ti substrate using the titanium inductively coupled plasma deep etch (TIDE) process (E620 R&D, Process conditions: 15 mT chamber pressure, 400 W ICP source power, 100 W substrate RF power, 100 sccm Cl2, and 5 sccm Ar) (Parker et al. 2005). The samples were then subjected to a final short dry etch to remove the remaining thin dielectric layer protecting the contact pads and recording sites, and released from the carrier by soaking in acetone. Scanning electron micrographs of a typical completed device are shown in Fig. 4. The smooth vertical sidewalls resulting from the TIDE process are clearly evident, as is the integrity of the dielectric and metal layers deposited on the titanium substrate.

Packaging

The microelectrode devices were packaged by bonding to commercially-available printed circuit boards (PCBs) (A-16, NeuroNexus Technologies) using cyanoacrylate adhesive (Pacer Technology, Rancho Cucamonga, CA). Gold wire-bonding was then used to make connections between the contact pads on the devices and their respective bond pads on the PCBs (7400A, West-Bond, Anaheim, CA). Afterwards, an additional layer of cyanoacrylate was applied over the contact pad area as an encapsulant to protect the exposed wires.

In situ recording site cleaning

After device fabrication and packaging was completed, intermittent contamination of the recording sites was observed on a number of devices during optical inspection, an example of which is shown in Fig. 5(a). Although the exact nature of this contamination is not known, it is believed to be residual dielectric not cleared by the final dry etch. As shown in Fig. 6, measurements performed using the in vitro testing apparatus described in Section 3.2 indicated that this contamination led to undesirably high impedance and low charge carrying capacity. As such, most devices were subjected to a 1 min, 1.5 V DC pulse using the in vitro testing apparatus. The resulting electrolysis at the recording sites facilitated residue removal, as evidenced by increased reflectivity of the cleaned site shown in Fig. 5(b). The cleaning process typically improved site performance, as evidenced by the reduced impedance and increased charge carrying capacity shown in Fig. 6. This in vitro recording site cleaning process is similar to those that have been performed during in vivo studies with shorter pulse duration (Otto, Johnson and Kipke 2006, Johnson, Otto and Kipke 2005).

Testing
Critical buckling force measurement

The buckling behavior of the microelectrode devices was assessed by longitudinal uniaxial compression testing. Both titanium devices and commercially-available silicon devices (A1 × 16–5 mm 100–413, NeuroNexus Technologies) were tested, the latter for performance benchmarking purposes. The devices were mounted to a silicon carrier chip using cyanoacrylate adhesive or double-sided carbon tape. The mounted devices were then attached to a manually-driven micromanipulator (M3301R, World Precision Instruments Inc., Sarasota, FL), which was used to load the device tips against a microbalance scale (AB54-S/FACT, Mettler Toledo, Columbus, OH). Forces exerted by the tips of the devices during testing were recorded using the microbalance (Rousche et al. 2001) and the devices were carefully observed for buckling and fracture via a CCD with magnifying optics. Five microelectrodes of the same design variant were tested for each length (i.e. Variant 3-L = 2 mm; Variant 9-L = 4.9 mm; and Variant 18-L = 5.4 mm).

In vitro functional characterization

The electrical performance of the microelectrode devices and the effect of plastic deformation on recording functionality were assessed in vitro using electrochemical impedance spectroscopy (EIS) and cyclic voltammetry (CV). In these studies, only titanium devices were tested, since silicon-based devices would be expected to fail catastrophically and, therefore, lose all recording functionality. Packaged devices were tested using the three-electrode test apparatus schematically illustrated in Fig. 7. The microelectrode-bearing PCB was connected to a wiring harness attached to ribbon cabling leading to an Autolab potentiostat PGSTAT12 (EcoChemie, Utrecht, The Netherlands) with built-in frequency analyzer (Brinkmann, Westbury, NY) (Pierce et al. 2009). The wiring harness was affixed to a manually-operated manipulator that allowed variation of the distance between the microelectrode tip and the bottom of the glass beaker. A calomel electrode (Fisher Scientific, Waltham, MA) was used as the reference electrode with a platinum wire serving as the counter electrode. Measurements were taken with the microelectrode immersed in 1X phosphate-buffered saline (PBS) solution at room temperature. The test apparatus was isolated within a copper mesh “Faraday” cage (not shown in Fig. 7). A 25 mV RMA sine wave was applied to electrode sites for EIS tests with frequencies ranging logarithmically from 0.1 to 10 kHz. CV testing was performed using a linear voltage sweep from −0.6 V to 0.8 V with a scanning rate of 1 V/s.

Functional characterization was first performed with the microelectrode tip positioned well above the floor of the glass beaker to establish baseline device performance (i.e. Measurement #1–Unloaded, undeformed state). Afterwards, the harness holding the PCB was manually lowered until the microelectrode tip came into contact with the bottom of the beaker, thereby imposing longitudinal uniaxial compression. The harness was then lowered further until elastic buckling was observed, at which point the harness position was fixed and EIS and CV measurements were taken again (i.e. Measurement #2–Loaded, elastically buckled state). The harness was then further lowered until plastic deformation of the devices was induced (as verified by permanent deformation after unloading). Afterwards, the harness was raised sufficiently to fully unload the plastically-deformed device, and further EIS and CV measurements were made (i.e. Measurement #3–Unloaded, plastically deformed state). Two to three samples of each device length were tested.

In vivo recording

Preliminary acute in vivo recordings were performed in a rat model. As described in greater detail elsewhere (McCarthy et al. 2011), a male Long-Evans rat was chosen, weighed, and placed under anesthesia. A midline incision was made through the scalp and the muscles were retracted. A head holder mount was constructed to stabilize the rat’s skull during subsequent microelectrode insertion and testing. The skull over the primary auditory cortex of the right hemisphere was then drilled using a burr and the exposed area was cleaned and prepared for device insertion. The microelectrode array was inserted through the intact dura mater into the cortical mantle (i.e. dura was not retracted). Broadband acoustic noise stimuli were then administered and electrophysiological recording was performed through the connection of an external pre-amplifier (Tucker-Davis Technologies, Alachua, FL) connected to the microelectrode PCB. The pre-amplifier digitized and transmitted the neural signals to a neural recording system for amplification, analysis, and storage. All animal procedures complied with guidelines for the care and use of laboratory animals and were approved by the Purdue Animal Care and Use Committee.

Results
Critical buckling force testing results

The average critical buckling forces of the titanium microelectrode devices were measured to be 19.41 ± 4.41, 20.88 ± 4.18, and 99.80 ± 20.70 mN for the 5.4, 4.9, and 2.0 mm length devices, respectively. In contrast, the average measured elastic buckling load for five 5 mm shank length commercially-available silicon devices was observed to be 3.1 ± 0.65 mN. Figure 8 plots the average buckling loads and standard deviations for titanium microelectrodes of varying designs and lengths relative to theoretical critical buckling loads, Pcr, estimated using Eulerian buckling analysis, which models the microelectrodes as long, slender columns under uniaxial longitudinal compressive loading (Rousche et al. 2001, Najafi, Ji and Wise 1990, Parker et al. 2007):

[Formula ID: Equ1]
[\documentclass[12pt]{minimal} \usepackage{amsmath} \usepackage{wasysym} \usepackage{amsfonts} \usepackage{amssymb} \usepackage{amsbsy} \usepackage{mathrsfs} \usepackage{upgreek} \setlength{\oddsidemargin}{-69pt} \begin{document}$${{\hbox{P}}_{\rm{cr}}} = \frac{{{{\pi }^2}{\text{EI}}}}{{{\hbox{L}}_{\rm{e}}^2}}$$\end{document}]
[Formula ID: Equ2]
[\documentclass[12pt]{minimal} \usepackage{amsmath} \usepackage{wasysym} \usepackage{amsfonts} \usepackage{amssymb} \usepackage{amsbsy} \usepackage{mathrsfs} \usepackage{upgreek} \setlength{\oddsidemargin}{-69pt} \begin{document}$${\hbox{I}} = \frac{{{\text{w}}{{\text{t}}^3}}}{{{12}}}$$\end{document}]
where E is the elastic modulus (ESi = 166 GPa (Senturia 2004); ETi = 107 GPa (Callister 2003)), I the moment of inertia, Le the effective shank length, w the shank width, and t the shank thickness. Effective shank length is dictated by the choice of end support conditions, with previous studies demonstrating fixed-free or fixed-pinned conditions as the most appropriate for the given experimental conditions (Najafi et al. 1990, Parker et al. 2007). As such, critical bucking load estimations were performed for each device length with Le= 2L (fixed-free) and Le= 0.7L (fixed-pinned), where L was taken to be the actual device shank length.

To simplify calculation of the theoretical critical bucking loads reported in Fig. 8, the tapered device shanks were approximated as uniform columns, i.e. columns with constant modulus, thickness, and width. The effective shank width was defined to be that which was necessary to maintain equivalent planar shank area for a given shank length. The shank thickness was defined as the sum of the thicknesses of the Ti foil used for the device fabrication and the dielectric layer stack (~ 1.5 μm). Although vendor specifications for the Ti foil indicated 25.4 μm nominal thickness, scanning electron microscope measurements performed on selected devices indicated actual thicknesses ranging from 34.2 to 37.6 μm with an average thickness of 35.2 μm (including dielectric stack), which slightly exceeds the stated manufacturing tolerance. As such, the experimentally measured average thickness was used for critical buckling load estimates. Finally, the elastic modulus of the column material was simply taken to be that of titanium, since the contribution of the dielectric layer stack would be minimized by its small thickness relative to the Ti substrate, and the relatively small modulus mismatch between Ti and the stack’s major constituents (i.e. ESiO2 = 70 GPa (Beer, Johnston and DeWolf 2002) and EAu = 80 GPa (Campbell 2001)). Although not reported here, finite element analyses performed for selected design variants with true device dimensions demonstrated excellent agreement with analytical solutions, thus suggesting that the underlying simplifying assumptions used for the analytical solutions did not introduce significant error.

In vitro functional characterization results

Measured EIS results for the titanium devices in the unloaded, undeformed state (i.e. measurements made with the device suspended in the in vitro characterization apparatus prior to mechanical loading against the beaker floor) indicated impedance values between 0.20 and 0.43 MΩ at 1 kHz frequency for recording site diameters of 40 μm, while a range of 0.75–1.38 MΩ was found for recording site diameters of 23 μm. Measured CV results revealed maximum charge carrying capacities ranging from 0.1 to 1.9 mC/cm2 for all design variants.

Figure 9 shows results from EIS and CV measurements for a single 23 μm recording site located near the middle of the tensile face of a 2 mm length titanium microelectrode device in the: a) unloaded, undeformed state; b) loaded, elastically deformed state; and c) unloaded, plastically deformed state. Increased impedance between the undeformed and deformed states suggests degradation of recording performance. Table 1 gives the average measured charge carrying capacities and impedances of ten similar 23 μm recording sites from two different devices for each of the loading states. While failure to perform in situ recording site cleaning in these devices resulted in significant scatter, similar recording performance trends were observed. Moreover, while most devices were observed to buckle such that tensile stress was imposed on the dielectric stack, similar trends in performance degradation were observed for devices in which buckling resulted in imposition of compressive stress upon the dielectric stack.

Figure 10 shows scanning electron micrographs of titanium microelectrodes imaged after plastic deformation within the in vitro functional characterization apparatus for devices in which the recording sites and traces were observed to lie on the tensile face (a & b) or the compressive face (c & d) of the device. Although the manual control of device displacement and absence of load recording capability during these tests precluded quantitative correlation of the degree of damage with imposed load or strain, the micrographs clearly demonstrate that dielectric cracking occurred during plastic deformation of the titanium shank, as would be expected due to the low toughness of the dielectric materials. However, the micrographs indicate that despite this damage, there is minimal evidence of dielectric loss and debris generation, at least within the experimental conditions explored during the current study.

In vivo recording results

Despite their significant length, the titanium microelectrodes were able to penetrate the dura mater, due to an increased cross-sectional area relative to commercially-available silicon-based microelectrodes. Figure 11 shows a recording trace from a single microelectrode site implanted in the auditory thalamus of an anesthetized rat (Device configuration: 5.4 mm shank length, 23 μm diameter sites, and 100 μm pitch). There was an easily isolatable action potential within the electrophysiologic data. The signal-to-noise ratio was 6.64, which is comparable to “good” recordings from conventional silicon-based microelectrode arrays (Suner et al. 2005).

Discussion
Buckling behavior

Assessment of buckling behavior was performed with the primary intent of ensuring that the titanium microelectrodes possessed sufficient stiffness for penetration of rat cortex, prior to undertaking in vivo studies. This was confirmed by observation of buckling loads for all device design variants (range = 12.26–132.35 mN) that were well in excess of the ~ 1 mN insertion force reportedly required for insertion of silicon microelectrodes with comparable design into rat cortex (Jensen, Yoshida and Hofmann 2006). This, therefore, suggests that the titanium microelectrodes will be able to sustain insertion forces many times greater than those expected in vivo.

The experimental measurements suggest that the tested silicon-based devices also possess sufficient stiffness for cortical insertion, although their margin of safety is significantly reduced relative to the Ti devices (measured buckling load range = 1.85 mN to 4.10 mN). The increased buckling resistance observed in titanium-based microelectrodes relative to the silicon-based devices can be largely explained by their increased thickness (~35 μm for Ti devices vs. ~15 μm for Si devices), which produces significant increase in moment of inertia, due to cubic dependence on thickness (Eq. 2). However, if silicon and titanium-based devices with equivalent dimensions (i.e. w, t, and Le) are compared, the following relationship emerges:

[Formula ID: Equ3]
[\documentclass[12pt]{minimal} \usepackage{amsmath} \usepackage{wasysym} \usepackage{amsfonts} \usepackage{amssymb} \usepackage{amsbsy} \usepackage{mathrsfs} \usepackage{upgreek} \setlength{\oddsidemargin}{-69pt} \begin{document}$${{\hbox{P}}_{\rm{Ti}}} = \frac{{{{\text{E}}_{\rm{Ti}}}}}{{{{\hbox{E}}_{\rm{Si}}}}}{{\hbox{P}}_{\rm{Si}}}$$\end{document}]

As can be seen, the critical buckling loads for titanium and silicon-based devices can be related through the ratio of their elastic moduli. Substitution of appropriate moduli values into Eq. 3 reveals that the predicted critical buckling load for a titanium microelectrode would be approximately 66% of a comparable silicon device.

While reduced buckling resistance implies reduced insertion performance relative to silicon, the observation of graceful failure via plastic deformation indicates potential for additional load bearing capacity beyond the onset of elastic buckling, thus forestalling fracture, often significantly. This is evidenced in the current study, as well a prior study of titanium microneedles with similar geometry (Parker et al. 2007), by the absence of fracture-based failure in any titanium device, even those tested well beyond the elastic buckling limit. The intrinsic brittleness of silicon, in contrast, largely precludes plasticity, thus resulting in onset of fracture soon after the elastic buckling limit has been exceeded, as was observed during testing of the silicon devices in the current study. As such, titanium microelectrodes provide greater tolerance to overloading during insertion and largely preclude potential for catastrophic fragmentation within the brain, thus increasing potential for enhanced reliability and safety relative to conventional silicon devices.

The data presented in Fig. 8 suggest that neither fixed-pinned nor fixed-free end conditions accurately model the experimentally measured buckling loads for the titanium microelectrode devices, although there is slight bias towards the latter. This may be partly explained by potential for minor slippage between the device tip and the smooth surface of the silicon chip (RA < 1 nm RMS) and/or the chip and the microbalance plate. While there were no observations of gross tip slippage during testing, the limited spatial resolution of the imaging system may have precluded observation of less pronounced slippage. Furthermore, manual control of device displacement during testing reduced the accuracy with which the critical buckling load could be determined, thus introducing potential for additional error. However, despite these limitations, the measured data demonstrate that the analytical solutions (and their underlying simplifying assumptions) can be used to estimate the bounds within which buckling is expected, at least within the design space considered in the current study.

In vitro recording behavior

Assessment of electrical performance was primarily performed with the intent of ensuring that the titanium devices provided sufficient recording performance, prior to undertaking in vivo studies. This was confirmed by measurement of impedances for devices in the unloaded, undeformed state (40 μm diameter site range = 0.20–0.43 MΩ; 23 μm diameter site range = 0.75–1.38 MΩ) that were in good agreement with specified values for silicon-based commercial devices (range = 0.5–3.0 MΩ, depending on the recording site diameter (Paralikar and Clement 2008)). Similarly, measured charge carrying capacities (range = 0.1–1.9 mC/cm2) were observed to be in fair agreement with silicon devices reported in the literature which utilize gold recording sites of similar sizes (Wise et al. 2004).

A secondary intent of the in vitro characterization studies was to determine whether titanium microelectrodes were able to maintain recording functionality after being subjected to elastic buckling or plastic deformation. The inability to accurately measure either load or displacement during these studies precluded systematic and quantitative analysis of the effect of deformation on recording performance. However, the data shown in Fig. 9 qualitatively demonstrate that titanium microelectrodes are able to retain a significant portion of their original recording functionality during elastic buckling, as well as after plastic deformation and unloading. Silicon devices were not tested in these studies, but it is reasonable to expect that their brittleness would severely limit possibility for continued recording functionality beyond elastic buckling, since fracture would soon follow. As such, this suggests that titanium microelectrodes may provide greater recording reliability relative to silicon devices, since some level of recording functionality can be retained despite overloading.

Definitive elucidation of the mechanisms underlying the degradation of recording performance with device deformation is beyond the scope of the current study. However, the scanning electron micrographs shown in Fig. 10 suggest that low dielectric fracture toughness results in accumulation of damage within the dielectric stack, e.g. cracking or delamination. Concomitant damage to the gold traces and recording sites would also be expected, e.g. plasticity, cracking, and/or delamination from the dielectric at severe strains. These types of damage would be expected to have increasingly detrimental effect on the recording performance. Although the observation of increased impedance with deformation supports this presumption, further study is required for validation. Nevertheless, when coupled with the plastic failure mode of the underlying titanium shank, the observed retention of the damaged dielectric suggests potential for an added degree of safety during insertion, relative to silicon-based devices. The degree of deformation required to produce such damage would be immediately apparent during the insertion attempt and would most likely occur prior to actual penetration. As such, opportunity would be provided for unloading and removal of the damaged device with minimal danger of fragmentation or debris generation, thus minimizing potential for adverse effect upon surrounding neural tissue, aside from trauma associated with compressive dimpling of the cortical surface during the attempted insertion. This stands in contrast to brittle silicon-based devices, whose failure under buckling presents potential for generation of numerous atomically-sharp fragments, both large and small.

Finally, although less likely, it is conceivable that titanium-based devices could be subjected to mechanical overloading once inserted. In such cases, dielectric cracking could result in eventual debris generation within the brain, due to potential for delamination produced by penetration of physiological fluids into the cracks. While the magnitude and severity of such debris would be far less than that associated with fracture of a comparable silicon-based device, this represents a potential concern nonetheless. Replacement of the current brittle dielectrics with ductile polymers could provide one means for addressing this concern. Polyimide represents an attractive candidate in this regard, due to its demonstrated biocompatibility in neural implantation applications (Richardson, Miller and Reichert 1993, Stieglitz and Meyer 1999, Rubehn and Stieglitz 2010). The use of polyimide as the structural basis for neural prostheses (Rousche et al. 2001, Stieglitz and Gross 2001), as well as flexible cabling for such devices (Hetke, Najafi and Wise 1990), has been demonstrated. However, the coupling of polyimide with titanium (as the primary structural component) would offer means for improving insertion reliability and recording site placement accuracy while minimizing shank cross section area.

In vivo recording

Assessment of in vivo performance was primarily performed with the intent of validating cortical penetration capability of the titanium microelectrodes, as well their acute neural recording capability. The preliminary in vivo results confirmed that titanium microelectrodes possessed sufficient stiffness to penetrate not only rat pia, but also dura, which is typically retracted prior to insertion of commercially-available silicon devices. Moreover, initial in vivo studies generated isolatable action potentials with signal to noise ratios comparable to commercially-available silicon-based devices. Subsequent studies have also demonstrated capability for simultaneous acute recording from both auditory cortex and thalamus from the same microelectrode (McCarthy et al. 2011). To the best of our knowledge, this represents the first such measurement made using a single microelectrode device. As discussed earlier, this capability may provide significant opportunity for facilitating studies targeted towards enhancing understanding of sequentially interconnected neural processing networks.

While these results are promising, chronic implantation studies are needed to assess long-term device stability and recording reliability. Such studies may highlight need for consideration of additional or alternative dielectric materials, such as amorphous silicon carbide and silicon oxycarbide, which have been shown to provide superior chemical stability and impermeability relative to SiO2 and Si3N4 in physiological saline environments (Cogan et al. 2003). They may also demonstrate need for consideration of recording site coatings, such as sputtered iridium oxide, which have been shown to provide significantly lower impedance than noble metals (Cogan, Plante and Ehrlich 2004). Finally, and perhaps most importantly, such studies are also likely to demonstrate need for integration of means for mitigating reactive tissue response (i.e. gliosis), which often degrades recording quality with time (Williams, Rennaker and Kipke 1999, Vetter et al. 2004, Williams et al. 2007). Use of titanium rather than silicon as the structural backbone for microelectrode devices is unlikely to provide benefit in this regard, since such substitution does not address the presumed mechanisms underlying reactive tissue response, i.e. implantation-induced injury and/or mechanical impedance mismatch with the surrounding tissue. However, numerous strategies have been proposed within this context, including pharmacological intervention (Shain et al. 2003, Kim and Martin 2006, Zhong and Bellamkonda 2007), surface modification (Wadhwa, Lagenaur and Cui 2006, Moxon et al. 2004a, Abidian and Martin 2009), and novel device design (Seymour and Kipke 2007, Kipke et al. 2008, Muthuswamy et al. 2005). The unique capabilities afforded by titanium micromachining, coupled with the favorable properties of titanium, may prove particularly advantageous for implementation of such strategies.

Conclusion

We have reported the design, fabrication, mechanical testing, in vitro, and in vivo characterization of titanium-based, “Michigan” type, penetrating microelectrodes for acute neural recording in rat. Mechanical testing results demonstrate that these devices posses sufficient stiffness for reliable cortical penetration, and also demonstrate that they provide potential for greater mechanical reliability and safety relative to current commercially-available silicon devices, due to their graceful, plasticity-based failure mode. In vitro characterization studies demonstrate that the titanium devices provide recording performance comparable to that of silicon-based devices, and also demonstrate that they provide potential for greater recording reliability, since plasticity-based failure allows maintenance of a significant degree of recording functionality despite overloading. Finally, results from preliminary in vivo studies corroborate many of these findings by demonstrating capability for reliable cortical insertion and acute recording with good signal to noise. Collectively, these results demonstrate the potential embodied in titanium as a promising new structural material for penetrating microelectrodes.

Acknowledgment

The authors would like to thank the Center for Neural Communication Technology for providing the silicon microelectrodes (NIH/NIBIB P41-EB002030). The authors also thank the staff at the Birck Nanotechnology Center (Purdue University) for assistance in device fabrication, and R. Madangopal and the students of the NeuroProstheses Research Laboratory (Purdue University) for assistance with in vitro characterization. Finally, the authors acknowledge support provided by the Cordier Fellowship Program (School of Mechanical Engineering, Purdue University), the Purdue Research Foundation, and the Showalter Research Trust (Purdue University).

Open Access This article is distributed under the terms of the Creative Commons Attribution Noncommercial License which permits any noncommercial use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.

References
 Abidian MR,Martin DC. Multifunctional nanobiomaterials for neural interfacesAdv Funct MaterYear: 20091957358510.1002/adfm.200801473 Aimi MF,Rao MP,Macdonald NC,Zuruzi AS,Bothman DP. High-aspect-ratio bulk micromachining of titaniumNat MaterYear: 2004310310510.1038/nmat105814743212 Bak MJ,Girvin JP,Hambrecht FT,Kufta CV,Loeb GE,Schmidt EM. Visual sensations produced by intracortical microstimulation of the human occipital cortexMed Biol Eng ComputYear: 19902825725910.1007/BF024426822377008 Beer FP,Johnston ER,DeWolf JT. Mechanics of materialsYear: 2002New YorkMcGraw-Hill Callister WD. Materials science and engineering : An introductionYear: 2003New YorkWiley Campbell SA. The science and engineering of microelectronic fabricationYear: 2001New YorkOxford University Press Chan H-Y,Aslam D,Wiler J,Casey B. A novel diamond microprobe for neuro-chemical and electrical recording in neural prosthesisJ Microelectromech SYear: 20091812 Cogan SF,Edell DJ,Guzelian AA,Liu YP,Edell R. Plasma-enhanced chemical vapor deposited silicon carbide as an implantable dielectric coatingJ Biomed Mater Res AYear: 200367A85686710.1002/jbm.a.1015214613234 Cogan SF,Plante TD,Ehrlich J. Sputtered iridium oxide films (SIROFs) for low-impedance neural stimulation and recording electrodesConference Proceedings of the IEEE Engineering in Medicine and Biology SocietyYear: 2004641536 Fanselow EE,Nicolelis MAL. Behavioral modulation of tactile responses in the rat somatosensory systemJ NeurosciYear: 1999197603761610460266 Fofonoff TA,Martel SM,Hatsopoulos NG,Donoghue JP,Hunter IW. Microelectrode array fabrication by electrical discharge machining and chemical etchingIEEE Trans Biomed EngYear: 20045189089510.1109/TBME.2004.82667915188855 Gelbard-Sagiv H,Mukamel R,Harel M,Malach R,Fried I. Internally generated reactivation of single neurons in human hippocampus during free recallScienceYear: 20083229610110.1126/science.116468518772395 Hetke JF,Najafi K,Wise KD. Flexible miniature ribbon cables for long-term connection to implantable sensorsSensor Actuat A-PhysYear: 199023999100210.1016/0924-4247(90)87076-U Hochberg LR,Serruya MD,Friehs GM,Mukand JA,Saleh M,Caplan AH,Branner A,Chen D,Penn RD,Donoghue JP. Neuronal ensemble control of prosthetic devices by a human with tetraplegiaNatureYear: 200644216417110.1038/nature0497016838014 Hubel DH,Wiesel TN. Laminar and columnar distribution of geniculo-cortical fibers in macaque monkeyJ Comp NeurolYear: 197214642145010.1002/cne.9014604024117368 Jensen W,Yoshida K,Hofmann UG. In-vivo implant mechanics of flexible, silicon-based ACREO microelectrode arrays in rat cerebral cortexIEEE Trans Biomed EngYear: 20065393494010.1109/TBME.2006.87282416686416 Johnson MD,Otto KJ,Kipke DR. Repeated voltage biasing improves unit recordings by reducing resistive tissue impedancesIEEE Trans Neural Syst Rehabil EngYear: 20051316016510.1109/TNSRE.2005.84737316003894 Kim DH,Martin DC. Sustained release of dexamethasone from hydrophilic matrices using PLGA nanoparticles for neural drug deliveryBiomaterialsYear: 2006273031303710.1016/j.biomaterials.2005.12.02116443270 Kipke DR,Shain W,Buzsaki G,Fetz E,Henderson JM,Hetke JF,Schalk G. Advanced neurotechnologies for chronic neural interfaces: New horizons and clinical opportunitiesJ NeurosciYear: 200828118301183810.1523/JNEUROSCI.3879-08.200819005048 Lee K,He J,Clement R,Massia S,Kim B. Biocompatible benzocyclobutene (BCB)-based neural implants with micro-fluidic channelBiosens BioelectronYear: 20042040440710.1016/j.bios.2004.02.00515308247 Lee KK,He JP,Singh A,Massia S,Ehteshami G,Kim B,Raupp G. Polyimide-based intracortical neural implant with improved structural stiffnessJ Micromech MicroengYear: 200414323710.1088/0960-1317/14/1/305 P.T. McCarthy, R. Madangopal, K.J. Otto, M.P. Rao. Titanium-based multi-channel, micro-electrode array for recording neural signals. In 31st Annual International Conference of the IEEE Engineering in Medicine & Biology Conference. Minneapolis, MN, 2009 P.T. McCarthy, M.P. Rao, K.J. Otto. Simultaneous recording of rat auditory cortex and thalamus via a titanium-based multi-nucleus, microelectrode array. submitted to Journal of Neural Engineering (2011) Motta PS,Judy JW. Multielectrode microprobes for deep-brain stimulation fabricated with a customizable 3-D electroplating processIEEE Trans Biomed EngYear: 20055292393310.1109/TBME.2005.84522515887542 Moxon KA,Kalkhoran NM,Markert M,Sambito MA,McKenzie JL,Webster JT. Nanostructured surface modification of ceramic-based microelectrodes to enhance biocompatibility for a direct brain-machine interfaceIEEE Trans Biomed EngYear: 20045188188910.1109/TBME.2004.82746515188854 Moxon KA,Leiser SC,Gerhardt GA,Barbee KA,Chapin JK. Ceramic-based multisite electrode arrays for chronic single-neuron recordingIEEE Trans Biomed EngYear: 20045164765610.1109/TBME.2003.82103715072219 Muthuswamy J,Okandan M,Gilletti A,Baker MS,Jain T. An array of microactuated microelectrodes for monitoring single-neuronal activity in rodentsIEEE Trans Biomed EngYear: 2005521470147710.1109/TBME.2005.85147816119243 Najafi K,Ji J,Wise KD. Scaling limitations of silicon multichannel recording probesIEEE Trans Biomed EngYear: 19903711110.1109/10.436052303265 Nicolelis MA,Shuler M. Thalamocortical and corticocortical interactions in the somatosensory systemProg Brain ResYear: 20011309011011480292 Nicolelis MAL,Baccala LA,Lin RCS,Chapin JK. Sensorimotor encoding by synchronous neural ensemble activity at multiple levels of the somatosensory systemScienceYear: 19952681353135810.1126/science.77618557761855 Normann RA. Technology insight: Future neuroprosthetic therapies for disorders of the nervous systemNat Clin Pract NeurolYear: 2007344445210.1038/ncpneuro055617671522 Otto KJ,Rousche PJ,Kipke DR. Cortical microstimulation in auditory cortex of rat elicits best-frequency dependent behaviorsJ Neural EngYear: 20052425110.1088/1741-2560/2/2/00515928411 Otto KJ,Rousche PJ,Kipke DR. Microstimulation in auditory cortex provides a substrate for detailed behaviorsHear ResYear: 200521011211710.1016/j.heares.2005.08.00416209915 Otto KJ,Johnson MD,Kipke DR. Voltage pulses change neural interface properties and improve unit recordings with chronically implanted microelectrodesIEEE Trans Biomed EngYear: 20065333334010.1109/TBME.2005.86253016485763 Otto SR,Shannon RV,Wilkinson EP,Hitselberger WE,McCreery DB,Moore JK,Brackmann DE. Audiologic outcomes with the penetrating electrode auditory brainstem implantOtol NeurotolYear: 2008291147115410.1097/MAO.0b013e31818becb418931643 Paralikar KJ,Clement RS. Collagenase-aided intracortical microelectrode array insertion: Effects on insertion force and recording performanceIEEE Trans Biomed EngYear: 2008552258226710.1109/TBME.2008.92315018713695 Parker ER,Thibeault BJ,Aimi MF,Rao MP,MacDonald NC. Inductively coupled plasma etching of bulk titanium for MEMS applicationsJ Electrochem SocYear: 2005152C675C68310.1149/1.2006647 Parker ER,Rao MP,Turner KL,Meinhart CD,MacDonald NC. Bulk micromachined titanium microneedlesJ Microelectromechanic SysYear: 20071628929510.1109/JMEMS.2007.892909 Pierce AL,Sommakia S,Rickus JL,Otto KJ. Thin-film silica sol-gel coatings for neural microelectrodesJ Neurosci MethYear: 200918010611010.1016/j.jneumeth.2009.02.008 Richardson RR,Miller JA,Reichert WM. Polyimides as biomaterials: Preliminary biocompatibility testingBiomaterialsYear: 19931462763510.1016/0142-9612(93)90183-38399958 Rousche P,Pellinen D,Pivin DJ,Williams J,Vetter R,Kipke D. Flexible polyimide-based intracortical electrode arrays with bioactive capabilityIEEE Trans Biomed EngYear: 20014836137110.1109/10.91480011327505 B. Rubehn, T. Stieglitz. In vitro evaluation of the long-term stability of polyimide as a material for neural implants. Biomaterials 31 (2010) Schuettler M,Stiess S,King BV,Suaning GJ. Fabrication of implantable microelectrode arrays by laser cutting of silicone rubber and platinum foilJ Neural EngYear: 20052S121S12810.1088/1741-2560/2/1/01315876647 Senturia SD. Microsystem designYear: 2004New YorkSpringer Seymour JP,Kipke DR. Neural probe design for reduced tissue encapsulation in CNSBiomaterialsYear: 2007283594360710.1016/j.biomaterials.2007.03.02417517431 Shain W,Spataro L,Dilgen J,Haverstick K,Retterer S,Isaacson M,Saltzman M,Turner JN. Controlling cellular reactive responses around neural prosthetic devices using peripheral and local intervention strategiesIEEE Trans Neural Syst Rehabil EngYear: 20031118618810.1109/TNSRE.2003.81480012899270 Sherman SM,Guillery RW. The role of the thalamus in the flow of information to the cortexPhilos T Roy Soc BYear: 20023571695170810.1098/rstb.2002.1161 T. Stieglitz, M. Gross. Flexible BIOMEMS with electrode arrangements on front and back side as key component in neural prostheses and biohybrid systems. Transducers '01: Eurosensors Xv, Digest of Technical Papers, Vols 1 and 2, 358–361 (2001) Stieglitz T,Meyer JU. Implantable microsystems. Polyimide-based neuroprostheses for interfacing nervesMed Device TechnolYear: 199910283010623349 Stieglitz T,Beutel H,Schuettler M,Meyer JU. Micromachined, polyimide-based devices for flexible neural interfacesBiomed MicrodevicesYear: 2000228329410.1023/A:1009955222114 Suner S,Fellows MR,Vargas-Irwin C,Nakata GK,Donoghue JP. Reliability of signals from a chronically implanted, silicon-based electrode array in non-human primate primary motor cortexIEEE Trans Neural Syst Rehabil EngYear: 20051352454110.1109/TNSRE.2005.85768716425835 T. Suzuki, K. Mabuchi, S. Takeuchi. A 3D flexible parylene probe array for multichannel neural recording. In Neural Engineering, 2003. Conference Proceedings. First International IEEE EMBS Conference on, 154–156 (2003) Szarowski DH,Andersen MD,Retterer S,Spence AJ,Isaacson M,Craighead HG,Turner JN,Shain W. Brain responses to micro-machined silicon devicesBrain ResYear: 2003983233510.1016/S0006-8993(03)03023-312914963 Takeuchi S,Suzuki T,Mabuchi K,Fujita H. 3D flexible multichannel neural probe arrayJ Micromech MicroengYear: 20041410410710.1088/0960-1317/14/1/014 Takeuchi S,Ziegler D,Yoshida Y,Mabuchi K,Suzuki T. Parylene flexible neural probes integrated with microfluidic channelsLab ChipYear: 2005551952310.1039/b417497f15856088 Vetter RJ,Williams JC,Hetke JF,Nunamaker EA,Kipke DR. Chronic neural recording using silicon-substrate microelectrode arrays implanted in cerebral cortexIEEE Trans Biomed EngYear: 20045189690410.1109/TBME.2004.82668015188856 Wadhwa R,Lagenaur CF,Cui XT. Electrochemically controlled release of dexamethasone from conducting polymer polypyrrole coated electrodeJ Control ReleaseYear: 200611053154110.1016/j.jconrel.2005.10.02716360955 Ward MP,Rajdev P,Ellison C,Irazoqui PP. Toward a comparison of microelectrodes for acute and chronic recordingsBrain ResYear: 2009128218320010.1016/j.brainres.2009.05.05219486899 Williams JC,Rennaker RL,Kipke DR. Long-term neural recording characteristics of wire microelectrode arrays implanted in cerebral cortexBrain Res ProtocYear: 1999430331310.1016/S1385-299X(99)00034-3 Williams JC,Hippensteel JA,Dilgen J,Shain W,Kipke DR. Complex impedance spectroscopy for monitoring tissue responses to inserted neural implantsJ Neural EngYear: 2007441042310.1088/1741-2560/4/4/00718057508 Winer JA,Larue DT. Patterns of reciprocity in auditory thalamocortical connections–Study with horseradish-peroxidase and autoradiographic methods in the rat medial geniculate-bodyJ Comp NeurolYear: 198725728231510.1002/cne.9025702123571530 Wise KD,Anderson DJ,Hetke JF,Kipke DR,Najafi K. Wireless implantable microsystems: High-density electronic interfaces to the nervous systemProc IEEEYear: 200492769710.1109/JPROC.2003.820544 Zhong YH,Bellamkonda RV. Dexamethasone-coated neural probes elicit attenuated inflammatory response and neuronal loss compared to uncoated neural probesBrain ResYear: 20071148152710.1016/j.brainres.2007.02.02417376408

Figures
 [Figure ID: Fig1] Fig. 1  Schematic representation of a typical titanium microelectrode device designed for acute cortical recording in rat [Figure ID: Fig2] Fig. 2  Schematic representation of a typical titanium microelectrode device designed for acute auditory corticothalamic loop recording in rat [Figure ID: Fig3] Fig. 3  Fabrication process flow for titanium microelectrodes [Figure ID: Fig4] Fig. 4  Scanning electron micrographs of titanium microelectrodes at varying magnifications [Figure ID: Fig5] Fig. 5  Optical micrographs of recording site reflectivity: (a) before; and (b) after in vitro cleaning [Figure ID: Fig6] Fig. 6  Measured impedance and charge carrying capacity in a device with contaminated recording sites before and after in vitro cleaning [Figure ID: Fig7] Fig. 7  Schematic of the in vitro functional characterization apparatus [Figure ID: Fig8] Fig. 8  Plot of experimentally measured buckling loads for various titanium microelectrode design variants vs. theoretical Euler critical buckling loads for fixed-free and fixed-pinned end conditions. Experimental data points represent the average measured buckling load for 5 specimens. The standard deviations of the reported measurements for each design variant are 20.70 mN, 4.18 mN, and 4.41 mN for shank lengths of 2 mm, 4.9 mm, and 5.4 mm, respectively [Figure ID: Fig9] Fig. 9  Results from EIS (top) and CV (bottom) testing of a titanium microelectrode device in: (a) unloaded, undeformed state; (b) loaded, elastically deformed state; and (c) unloaded, plastically deformed state. Both EIS and CV data were taken from the same recording site, which was located near the middle of the tensile face of the device [Figure ID: Fig10] Fig. 10  Scanning electron micrographs of typical examples of dielectric damage resulting from plastic deformation of titanium microelectrodes: (a) & (b) Typical surface morphologies near the middle of the shank of devices where the recording sites and traces were observed to lie on the tensile face; (c) & (d) Typical surface morphologies near the middle of the shank of devices where the recording sites and traces were observed to lie on the compressive face [Figure ID: Fig11] Fig. 11  Extracellular recording from auditory thalamus of an anesthetized rat

Tables
[TableWrap ID: Tab1] Table 1

Average measured charge carrying capacities and impedances of 23 μm recording sites during buckling testing of titanium microelectrodes (10 sites over 2 devices)

Loading State Charge Carrying Capacity (mC/cm2) Impedance (MΩ)
Unloaded, Undeformed 0.32 ± 0.10 1.51 ± 0.23
Loaded, Elastically Deformed 0.60 ± 0.22 1.83 ± 0.53
Unloaded, Plastically Deformed 0.53 ± 0.28 1.67 ± 0.51

 Article Categories:Article Keywords: Keywords MEMS, Prosthesis, Electrophysiology, Recording, Microstimulation, Brain-machine.

Previous Document:  Pioglitazone limits myocardial infarct size, activates Akt, and upregulates cPLA2 and COX-2 in a PPA...
Next Document:  Smoking and alcohol consumption in relation to risk of triple-negative breast cancer in a cohort of ...